Bonding of plastic pipe systems
The "chemical welding" by means of solvents or simply "BONDING", is a specially developed connection for pipes and fittings from PVC-U. Bonding is realized by means of adhesives, resulting from the solution of PVC-U polymer in an appropriate solvent. The adhesives soften the walls of the pipes and fittings, followed by "welding" with material contained in the walls. The "chemical welding" allows long-term bonds, which guarantee the same properties of chemical and mechanical resistance than the original pipes and fittings. The adhesives have to be selected depending on the type of resin, as the solvents and filler materials contained therin may vary. Please note that in a pipe system only adhesives from the same series are allowed to be used for the PVC-U pipes as well as for fittings and valves.
The adhesive used for bonding parts from the PVC-U system may in no case be used for bonding foreign parts.
Instructions for bonding
First of all, it is very important to check if the accessory parts are in good condition, especially have to be verified the flowability, the homogeneity of the adhesive and the expiration date.
Cut the pipe vertically. To obtain a good cut, it is recommended to use a suitable pipe cutter with rollers. Such an instrument is produced especially for cutting plastic pipes.
|Chamfer the outer surface of the pipe end, so that it can be inserted correctly into the fitting (angle 15°). This procedure is extremely important, as otherwise the adhesive may be scraped off, which can affect the quality of the connection and has to be done by means of particular chamfering devices.|
|Measure the depth of the gluing sleeve. Highlight the measured value on the pipe end.|
|Remove all traces of dirt or grease from the entire bonding length with a clean absorbant paper towel or with a brush moistened with cleaning agent. Repeat the same process on the inside area of the sleeve, in order to soften its surface.
Let the surfaces dry for some minutes, before applying the adhesive. The cleaning agent not only cleans the surfaces before bonding, but also has a softening effect and prepares the parts for the adhesive, in order to achieve an optimum bond.
|Spread the adhesive evenly and in longitudinal direction on the parts to be bond (outer surface of the pipe and inner surface of the gluing sleeve). Use a rough brush of appropriate size. In any case it is recommended to use a brush at least half as big as the diameter of the pipe.
Apply the adhesive on the entire length of the connecting surfaces of pipe and fitting:
- on the complete insertion depth up to the end stop
- on the total bonding area of the pipe (which has been previously marked outside).
Insert the pipe with the entire bonding length into the fitting, without twisting. Only after this process, both components can be rotated slightly (maximum rotation between pipe and fitting: 1/4 turn). By means of this rotation, the applied adhesive will be equalised.
|The bond between pipe and fitting must be completed very quickly (times longer than 20-25 seconds are to be avoided). Depending on the outer diameter of the pipe and the forces occuring, bonding of pipe and fitting has to be carried out as follows:
- outer diameter d < 90 mm by one person.
- outer diameter d 90 mm up to < 160 mm by two persons.
- outer diameter d > 160 mm with help of insert devices.
|Fix the parts for some seconds, immediately after having inserted the pipe into the fitting (until the end stop). Then remove the excess adhesive by means of crepe paper or cloth, if possible also from the inner surfaces.
Drying of the adhesive: It is very important to let the bonded parts rest for a while, in order to ensure a natural flash-off of the adhesive. Flash-off time depends on the stress, which the bond has to withstand later.
|The following minimum times at room temperature have to be observed,
before the bond can be strained:
- 5 to 10 minutes for ambient temperatures > 10°C
- 15 to 20 minutes for ambient temperatures < 10°C
pressure at repair weld not being subject to hydraulic tests, effective for all dimensions and pressures:
- 1 hour per bar
in the case of bonds being subject to hydraulic tests for pipes and fittings up to PN 16 and independent from the diameter, it is essential to wait:
- at least 24 hours.
Flash-off times of the adhesive depend on the room temperaure as well. In the event of special climate conditions (humidity, temperature, etc.) we recommend you to get in touch with our technical service and/or the manufacturer of the adhesive, in order to obtain further support.
Should the outer diameter of the pipe and the inner diameter of the fitting be near the limit of the tolerance range, the dry pipe may in no case be inserted into the dry gluing sleeve. This will only be possible after having applied cleaning agent and adhesive on the the two parts to be bond.
The adhesive has been produced from the same resin as the PVC-U, which the company FIP uses for manufacturing pipes, fittings and valves from the PVS-U system. Unless otherwise indicated, the adhesive has to cover the following tolerances:
- max. excess: 0,2 mm.
- max. gap: 0,6 mm.
When using the adhesive and the cleaning agents, it is advisable to respect the following instructions:
Wear safety gloves and safety glasses, in order to protect eyes and hands.
The adhesive and the cleaning agent may be used only in rooms with sufficient ventilation (they irritate airways and eyes).
Adhesive and cleaning agent contain solvents and because of their volatility, it is important to close the bins immediately after use.
Solvents in gaseous phase tend to form flammable gases. For this reason, all kinds of ignition sources have to be removed or avoided, such as welding operations, electrostatic charge and smoking. The instructions given by the manufacturer on the packaging have to be observed.
It is advisable to perform the bonding only at a temperature between + 5 and + 40° C, in order to ensure optimum adhesion.
Quantity of adhesive for one bonding depends on various factors (climate, dimensions of the pipe, viscosity of the adhesive, experience of the personnel, etc.), factors, which are not easy to evaluate.
INFORMATION TO OUR DELIVERY PROGRAM
Plastic pipe systems
Overview of plastic pipe systems
Technical information on ABS pipe systems
Technical information on PVC U pipe systems
Technical information on PVC U transparent pipe systems
Technical information on PVC C pipe systems
Technical information on PP pipe systems
Technical information on PP-R pipe systems
Technical information on PE pipe systems
Technical information on PVDF pipe systems
Chemiedur - pipe
Technical information on UP-GF (FRP) pipe systems
UP-GF (FRP) pipes
UP-GF (FRP) molded parts and connection
UP-GF-PP (FRP) molded parts and connection
UP-GF (FRP) adhesive collars
UP-GF (FRP) loose flanges
Pot Strainer DN 200 - DN 500 Inliner PP/FRP Coated
Pot Strainer DN 200 - DN 500 Inliner FRP/CBL Coated
Angle Seat Strainer DN 200 - DN 400 Inliner FRP/CBL Coated
Manhole mad of FRP and PP/FRP
Calculator for cutting pipes
Guidelines for sawing plastic pipe
Leftovers in plastic pipe
Standardization of plastic pipes and molded parts
PVC U pipes deviations
Pressure loss in pipe systems out of PVC U, PVC C and ABS pipe systems
Distinction between Rp, R and G threads
Screw lengths for flange connections
PVC U transparent ball valves
Plastic needle valves
Plastic Valves according to ATEX
New EU guideline 2014/34/EU
Plastic Valves in EX zones
Y-Strainers PP-EL DN 15 - DN 50
Check valves PP-EL DN 15 - DN 50
Angle seat valves PP-EL DN 15 - DN 50
Bonding of plastic pipes
Video showing the bonding of pipes
Guidelines for extrusion welding
Grids / support grids
Grids out of PP -el electrically conductive
Profile support grids out of PP -el electrically conductive
Molded ventilation parts
PVC transparent hose with fabric inlay
Industrial tanks and chemical containers
Dosing tanks and outer containers 35 1000 Liter
Salt dissolving tanks 60 -5000 Liter
Storage tanks and vats
Storage tanks for water
Safety and collecting troughs
Industrial tank delivery program
Dosing tanks with agitator
Dosing tank agitators
Dosing tanks with attachments
Dosing tanks made of sheet material
Customized chemical containers
Dosing tanks with level indicators
IBC screw caps DN 150/DN 200
IBC adapters out of PE
IBC adapters out of PP
MULTI FLEX BLOCK for IBC BULK CONTAINER
Attachment parts for tank construction
CO2 - absorbes
Filter housings and filter cartridges
PENTEK 3G Slime Line filter housings
PENTEK 3G Standard filter housings
PENTEK Big Blue filter housings
PENTEK PP high temperature filter housings
PENTEK PP all nature filter housings
PENTEK filter bags for Big Blue filter housings
PENTEK surface filter cartridges
PENTEK filter cartridges for depth filtration
PENTEK filter cartridges with activated carbon
CINTROPUR filter systems
CINTROPUR water filters
Blind flanges, loose flanges, rectangular flanges
Table of chemical resistance for plastic pipe systems
Machined plastic parts
Milled plastic parts
Loose flanges and blind flanges made of sheet material
Static mixers made of plastic
Single-type and double-type strainers
Pot strainer DN 300
Angle seat strainer DN 500
Variable area flow meters
Configuration tool for flow meters
Laboratory filter presses
Injection molded parts
Scraper made of PE for filter press
OUR - PREMIUM PARTNERS -